OPEN SUBJECT AREAS: MATERIALS CHEMISTRY
Touching polymer chains by organic field-effect transistors Wei Shao1,4, Huanli Dong1, Zhigang Wang2 & Wenping Hu1,3
Received 25 February 2014 Accepted 7 August 2014 Published 17 September 2014
Correspondence and requests for materials should be addressed to
Beijing National Laboratory for Molecular Sciences, Key Laboratory of Organic Solids, Institute of Chemistry, Chinese Academy of Sciences, Beijing 100190, China, 2Department of Polymer Science and Engineering, Hefei National Laboratory for Physical Sciences at the Microscale, University of Science and Technology of China, Hefei, Anhui 230026, China, 3Department of Chemistry, School of Science, Tianjin University and Collaborative Innovation Center of Chemical Science and Engineering (Tianjin), Tianjin 300072, China, 4Samsung R&D Institute China - Beijing (SRC-Beijing), Beijing 100028, China.
Organic field-effect transistors (OFETs) are used to directly ‘‘touch’’ the movement and dynamics of polymer chains, and then determine Tg. As a molecular-level probe, the conducting channel of OFETs exhibits several unique advantages: 1) it directly detects the motion and dynamics of polymer chain at Tg; 2) it allows the measurement of size effects in ultrathin polymer films (even down to 6 nm), which bridges the gap in understanding effects between surface and interface. This facile and reliable determination of Tg of polymer films and the understanding of polymer chain dynamics guide a new prospect for OFETs besides their applications in organic electronics and casting new light on the fundamental understanding of the nature of polymer chain dynamics.
Z.W. ([email protected]
. edu.cn) or W.H. ([email protected]
rganic field-effect transistors (OFETs) are a class of devices consisting of an organic semiconductor layer, a gate insulator layer and three terminals (drain, source and gate electrodes)1–3. Charges inject from the source electrode into organic semiconductor layer, and then transport through the organic semiconductor layer, and flow out at the drain electrode4. The route of charge transport in organic semiconductor layer is named conducting channel, which exists exactly at the interface between the organic semiconductor layer and the gate insulator layer5 with thickness of one to several molecular layers6. This molecular level conducting channel is highly sensitive to out stimulus, so that OFETs could be used as an ultra sensitive sensors or actuators for pressure7, chemical and biological detection8 etc. Facchetti et al. have made a pioneer study by using OFETs for surface viscoelastic properties of polymers depending on the correlation of device mobility and micro structural and morphological alterations of semiconductor layer on polymer9. It opens a door for the integration of organic electronics and polymer science, e.g., to face polymer chain dynamics (e.g., the glass transition dynamics)10, one of the difficult problems of polymer sciences in this century. The glass transition of a polymer is a reversible transition from a hard and relatively brittle state into a rubberlike state at the glass transition temperature (Tg). Therefore, Tg, corresponding to the movement and long-range transport of polymer chains, exhibiting the massive change in physical properties of a polymer, becomes a key and fundamental parameter of polymer science11. Many conventional methods, including ellipsometry12, Brillouin scattering13, X-ray reflectivity14, dielectric relaxation spectroscopy15 and fluorescence spectroscopy16, depending on changes of physical appearance at Tg rather than probing the characteristics of polymer chain dynamics, all the techniques are indirect. Here, we introduce a direct way to touch polymer chain dynamics by using OFETs as molecular level probes. It is a development of Facchetti et al.’s method10 by visualizing the abrupt current change of OFETs directly at the glass transition instead of the estimation of series mobilities of OFETs as the reference addressed10. In our experiments, OFETs are designed with bi-layer dielectrics (polymer/SiO2). The target polymer layer (e.g., polystyrene (PS)) is sandwiched between the organic semiconductor layer (e.g., copper phthalocyanine (CuPc)) and SiO2 gate insulator layer. CuPc was selected as the candidate due to its low cost, high thermal and chemical stability as well as excellent field-effect properties17,18. The results of current–temperature characteristics of OFETs with different PS molecular weights are shown in Figure 1 (left blue curves, and different molecular weights as shown in curves of a–d). It is attractive that all curves show two distinct regions, with the drain currents initially increasing with temperature increasing, and then decreasing at higher temperatures. When extrapolating the two tendencies to their intersection to get the transition point temperature, more attractively, the temperatures at these intersection points agree very well with the Tg values of the corresponding bulk polymers, which can
SCIENTIFIC REPORTS | 4 : 6387 | DOI: 10.1038/srep06387
Figure 1 | Current with abrupt changes in OFETs (left-hand blue curves) and corresponding DSC scans at Tg (right-hand black curves) for PS films with different molecular weights. The currents initially increase with temperature increasing, and then decreasing at higher temperatures (left blue curves). When extrapolating the two tendencies to their intersection to get the transition point temperature, which agree very well with the Tg values of the corresponding bulk polymers by DSC (right black curves).
be confirmed by differential scanning calorimetry (DSC) results (Figure 1, right black curves, and different molecular weights as shown in curves of a–d). Temperature-dependence Atomic force microscopy (AFM) images and in-situ X-ray diffraction (XRD) patterns of the CuPc layer in OFETs exhibit no obvious change (Figure 2 and Figure S1), indicating the morphology and microstructure of organic semiconductor layer are not responsible for the current transitions of the OFETs. Hence, the fundamental changes arising from the underlying polymer layer and the corresponding interface between organic semiconductor/polymer insulator should be responsible for such current transitions. It is worth noting that our method is different from Facchetti’s19,20, who correlated the device-performance trends to the evolution of organic semiconductor film morphology and microstructure, and empirically defined the glass transition temperature at which the TFT carrier mobility falls by 50%. If we assume charge transport in organic semiconductors is pursued by hopping21, i.e., charges pass from one molecule to another with the assistance of phonons. With temperature increasing, the thermal vibrations of phonons will increase, which promotes charge transport and leads to an increase of current. Simultaneously, the movement and dynamics of the underlying polymer chains will be enhanced. When temperature is below Tg, the charge transport in OFETs is located in a well-defined conducting channel at the interface between organic semiconductor and polymer insulator (Figure 3a,b). However, when temperature is above Tg, the polymer transforms from a hard and relatively brittle state into a rubber-like state, i.e., the chain segments shift from a ‘‘frozen in’’ or cessation state (the glassy state, T , Tg) to a cooperative motion state (the rubbery state, T $ Tg)22. Accompanied with this transformation, molecular motion and dynamics increase dramatically, typically by more than 10 orders of magnitude. This kind of cooperative motion of the polymer chains will result in the disruption of the perfect conducting channel (Figure 3c), and lower the current of the SCIENTIFIC REPORTS | 4 : 6387 | DOI: 10.1038/srep06387
Figure 2 | In-situ XRD scans for 70-nm-thick CuPc films on PS dielectric as a function of temperature. The peak of the CuPc film (Peak 1) is at 2h position of 6.9, corresponding to the a-phase. Additional peaks observed in the scans were from the background (Peak 2 and 3). Note that the peak position and intensity of the CuPc film are almost identical with the temperature increased to 373 K, indicating there is no obvious microstructure change in the selected temperature regime.
OFET significantly. Therefore, the current in an OFET will initially increase with temperature increasing (T , Tg) due to the phonon assisted charge transport, but then decrease at higher temperatures (T $ Tg) because of the disruption of the perfect conducting channel by the cooperative motion of polymer chains, i.e., the current transition arises from the fundamental change in molecular motion and dynamics that occurs at Tg. This is highly according with our results as shown in Figure 1, i.e., the conducting channel of OFETs provides a direct and vivid platform to ‘‘visualize’’ the movement and dynamics of polymer chains and then determine the values of Tg. In order to confirm the generality of this conclusion, other polymers, such as polylactide (PLA), polyacrylonitrile (PAN) and poly (methyl methacrylate) (PMMA), are also incorporated into OFETs to examine their current-temperature characteristics (Figure 4). Indeed, in all cases, the values of the intersection temperatures obtained from our OFETs are highly consistent with the Tg values of the corresponding bulk polymers. It confirms the generality of our method by using conducting channel of OFETs as a direct vivid platform to ‘‘touch’’ the movement and dynamics of polymer chains. Moreover, another unique feature of our OFETs is the distinctive nanometer-sized confined polymer layer, which provides a facile way to examine the effects of confinement during the glass transition process by selectively tuning the thickness of polymer layer. It is generally accepted that when the thickness of polymer films decreases to a scale comparable to the cooperative length of polymer itself, the conformation of polymer molecules becomes perturbed which eventually affects the properties of the polymer due to the nanometer-sized effect23,24, however, a quantitative understanding of perturbations to chain dynamics due to geometric constraints remains a challenge25,26. Here, our OFETs could fill in to do something. The results of our OFETs on the detection of polymer thickness dependence on Tg are shown in Figure 5. When PS films are relatively thin the values of Tg increase rapidly with film thickness, and then approach a constant gradually at 45–55 nm. This nanoconfined effect is probably attributed to the increasing molecular motion and dynamics with the thickness getting thinner11. Since the thickness of the polymer film is comparable to, or less than, the cooperative length scale of the polymer chains, the configuration and extent 2
Figure 3 | OFET structure and the conducting channel in OFETs. (a), OFET structure, conducting channel is formed at the interface between polymer and organic semiconductor. (b), electron transport in a prefect conducting channel below Tg, charge transport is located in a well-defined conducting channel. (c), electron hindered in a disrupted conducting channel, above Tg, the chain segments shift from a ‘‘frozen in’’ or cessation state (the glassy state, T , Tg) to a cooperative motion state (the rubbery state, T $ Tg).
of entanglement of polymer chains in the films will be different from those in the bulk. Our method offers the promise of understanding nanoconfined molecular dynamic behavior due to the advantage of easy confining film dimensions and varying the thickness. Moreover,
Figure 4 | Plots of drain current versus temperature for different polymers in OFETs (left-hand blue curves) and DSC scans for the corresponding polymers (right-hand black curves). (a), PLA, (b), PAN, (c,d), PMMA with different molecular mass. In all cases, the values of the intersection temperatures obtained were highly consistent with the DSC data of the corresponding bulk polymers. SCIENTIFIC REPORTS | 4 : 6387 | DOI: 10.1038/srep06387
it is worth noting that our method could detect the transition temperature and pinpointing the location of Tg even when the film thickness is ultrathin, as thin as 6 nm (Figure S2). This makes it significantly better than other currently available techniques with signals always discontinuous or below the noise level when measuring the Tg of ultra-thin polymer films. Finally, it is attractively to be noted that the facile detection of polymer chain dynamics by OFETs opens the door for micro devices to touch polymer chain dynamics (Figure S3). In summary, OFETs are used to directly ‘‘touch’’ the movement and dynamics of polymer chains, and then determine Tg. The conducting channel of OFETs exhibits several unique advantages: 1) it directly detects the dynamics of polymer chain at Tg, instead of
Figure 5 | Dependence of Tg values on film thickness for PS. Variation of Tg as a function of film thickness, the value of Tg increases rapidly with increasing film thickness, and then gradually approaches a constant value. 3
www.nature.com/scientificreports detecting changes in physical appearance as in the case of conventional techniques; 2) it allows the measurement of size effects in ultrathin polymer films (even down to 6 nm), which bridges the gap in understanding effects between surface and interface. This facile and reliable determination of Tg of polymer films and the understanding of polymer chain dynamics guide a new prospect for OFETs besides their applications in organic electronics and casting new light on the fundamental understanding of the nature of polymer chain dynamics, even the dependence of Tg on molecular mass and heating rates (Figure S4–S5) etc.
Methods Polystyrene (PS), poly(methyl methacrylate) (PMMA), polyacrylonitrile (PAN) and polylactide (PLA) were purchased from Aldrich Chemical Co. and used as received. Details of the used polymer samples are listed in Table S1. The OFETs were characterized using a Keithley 4200 Semiconductor Parameter Analyzer equipped with a temperature controller. Temperature-dependent OFET measurements were directly performed in air with the temperature regulated at a constant heating rate. The drain current data as a function of temperature were recorded in the saturation regimes with a fixed gate voltage and drain bias of 260 and 245 V, respectively. A ramp rate of 2.5 K/min was used in order to minimize any undesirable effects, such as the different coefficients of thermal expansion in the device components. At least three measurements were recorded at each temperature and statistically averaged values were calculated. The calorimetric Tg values for the bulk polymers were obtained by differential scanning calorimetry (DSC). Atomic force microscopy (AFM) and in-situ X-ray diffraction (XRD) were employed to determine the thickness of polymer thin films and to examine the film microstructures as a function of temperature. 1. Tsumura, A., Koezuka, H. & Ando, T. Macromolecular electronic device - fieldeffect transistor with a polythiophene thin-film. Appl. Phys. Lett. 49, 1210–1212 (1986). 2. Sirringhaus, H. et al. Two-dimensional charge transport in self-organized, highmobility conjugated polymers. Nature 401, 685–688 (1999). 3. Bao, Z. & Locklin, J. J. Organic field-effect transistors (CRC Press, 2007). 4. Hu, W. Organic Optoelectronics (Wiley-VCH, 2012). 5. Wang, C., Dong, H., Hu, W., Liu, Y. & Zhu, D. Semiconducting p-Conjugated Systems in Field-Effect Transistors: A Material Odyssey of Organic Electronics. Chem. Rev. 112, 2208–2267 (2012). 6. Jiang, L. et al. Millimeter-sized molecular monolayer two-dimensional crystals. Adv. Mater. 23, 2059–2063 (2011). 7. Mannsfeld, S. C. B. et al. Highly sensitive flexible pressure sensors with microstructured rubber dielectric layers. Nat. Mater. 9, 859–864 (2010). 8. Roberts, M. E. et al. Water-stable organic transistors and their application in chemical and biological sensors. PNAS 105, 12134–12139 (2008). 9. Kim, C., Facchetti, A. & Marks, T. J. Polymer gate dielectric surface viscoelasticity modulates pentacene transistor performance. Science 318, 76–80 (2007). 10. Debenedetti, P. G. & Stillinger, F. H. Supercooled liquids and the glass transition. Nature 410, 259–267 (2001). 11. Fakhraai, Z. & Forrest, J. A. Measuring the surface dynamics of glassy polymers. Science 319, 600–604 (2008). 12. Sharp, J. S. & Forrest, J. A. Free surfaces cause reductions in the glass transition temperature of thin polystyrene films. Phys. Rev. Lett. 91, 235701 (2003). 13. Forrest, J. A., DalnokiVeress, K., Stevens, J. R. & Dutcher, J. R. Effect of free surfaces on the glass transition temperature of thin polymer films. Phys. Rev. Lett. 77, 2002–2005 (1996). 14. Wallace, W. E., Vanzanten, J. H. & Wu, W. L. Influence of an impenetrable interface on a polymer galss-transition temperature. Phys. Rev. E 52, R3329–R3332 (1995).
SCIENTIFIC REPORTS | 4 : 6387 | DOI: 10.1038/srep06387
15. Fukao, K. & Miyamoto, Y. Glass transitions and dynamics in thin polymer films: dielectric relaxation of thin films of polystyrene. Phys. Rev. E 61, 1743–1754 (2000). 16. Ellison, C. J. & Torkelson, J. M. The distribution of glass-transition temperatures in nanoscopically confined glass formers. Nature Mater. 2, 695–700 (2003). 17. Bao, Z., Lovinger, A. J. & Dodabalapur, A. Organic field-effect transistors with high mobility based on copper phthalocyanine. Appl. Phys. Lett. 69, 3066–3068 (1996). 18. Zeis, R., Siegrist, T. & Kloc, C. Single-crystal field-effect transistors based on copper phthalocyanine. Appl. Phys. Lett. 86, 022103 (2005). 19. Kim, C., Facchetti, A. & Marks, T. J. Probing the surface glass transition temperature of polymer films via organic semiconductor growth mode, microstructure, and thin-film transistor response. J. Am. Chem. Soc. 131, 9122–9132 (2009). 20. Kim, C., Quinn, J. R., Facchetti, A. & Marks, T. J. Pentacene transitiors fabricated on photocurable polymer gate dielectrics: tuning surface viscoelasticity and device response. Adv. Mater. 22, 342–346 (2010). 21. Pope, M. & Swenberg, C. E. Electronic Processes in Organic Crystals and Polymers (Second Edition, Oxford University Press, 1999). 22. Gibbs, J. H. & DiMarzio, E. A. Nature of the glass transition and the glassy state. J. Chem. Phys. 28, 373–383 (1958). 23. Keddie, J. L., Jones, R. A. L. & Cory, R. A. Interface and surface effects on the glasstransition temperature in thin polymer-films. Faraday Discuss. 98, 219–230 (1994). 24. Priestley, R. D., Ellison, C. J., Broadbelt, L. J. & Torkelson, J. M. Structural relaxation of polymer glasses at surfaces, interfaces and in between. Science 309, 456–459 (2005). 25. Jones, R. L., Kumar, S. K., Ho, D. L., Briber, R. M. & Russell, T. P. Chain conformation in ultrathin polymer films. Nature 400, 146–149 (1999). 26. O’Connell, P. A. & McKenna, G. B. Rheological measurements of the thermoviscoelastic response of ultrathin polymer films. Science 307, 1760–1763 (2005).
Acknowledgments The authors acknowledge the financial support from National Natural Science Foundation of China (51033006, 51222306, 51003107, 91027043, 91222203, 91233205), the China-Denmark Co-project (60911130231), TRR61 (NSFC-DFG Transregio Project), the Ministry of Science and Technology of China (2011CB808400, 2013CB933403, 2013CB933500), the Chinese Academy of Sciences.
Author contributions W.H. and Z.W. conceived the research and designed the experiments. W.S. and H.D. fabricated the devices, performed the experiments and data analysis. All authors discussed the results and commented on the manuscript.
Additional information Supplementary information accompanies this paper at http://www.nature.com/ scientificreports Competing financial interests: The authors declare no competing financial interests. How to cite this article: Shao, W., Dong, H., Wang, Z. & Hu, W. Touching polymer chains by organic field-effect transistors. Sci. Rep. 4, 6387; DOI:10.1038/srep06387 (2014). This work is licensed under a Creative Commons Attribution-NonCommercialShareAlike 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder in order to reproduce the material. To view a copy of this license, visit http:// creativecommons.org/licenses/by-nc-sa/4.0/